The crystal structure described by Li4Mn3Cu3(SnO8)2 is Spinel-derived structured and crystallizes in the triclinic P1 space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(11), one O(12), one O(15), and one O(3) atom to form LiO4 tetrahedra that share  a cornercorner with one Mn(1)O6 octahedra,  a cornercorner with one Cu(1)O6 octahedra,  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Mn(2)O6 octahedra, corners with two equivalent Mn(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, and corners with three equivalent Sn(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 55-63°. In the second Li site, Li(2) is bonded in a rectangular see-saw-like geometry to one O(14), one O(16), one O(5), and one O(9) atom. In the third Li site, Li(3) is bonded in a rectangular see-saw-like geometry to one O(1), one O(10), one O(4), and one O(6) atom. In the fourth Li site, Li(4) is bonded to one O(13), one O(2), one O(7), and one O(8) atom to form LiO4 tetrahedra that share  a cornercorner with one Mn(2)O6 octahedra,  a cornercorner with one Mn(3)O6 octahedra,  a cornercorner with one Cu(3)O6 octahedra, corners with two equivalent Mn(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, and corners with three equivalent Sn(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 57-63°. There are three inequivalent Mn sites. In the first Mn site, Mn(1) is bonded to one O(14), one O(16), one O(3), one O(4), one O(7), and one O(8) atom to form MnO6 octahedra that share corners with two equivalent Sn(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Sn(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, and edges with two equivalent Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles are 52°. In the second Mn site, Mn(2) is bonded to one O(1), one O(10), one O(11), one O(13), one O(15), and one O(5) atom to form MnO6 octahedra that share corners with two equivalent Sn(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Sn(2)O6 octahedra, edges with two equivalent Mn(3)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-52°. In the third Mn site, Mn(3) is bonded to one O(10), one O(12), one O(13), one O(15), one O(5), and one O(6) atom to form MnO6 octahedra that share corners with two equivalent Sn(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Sn(2)O6 octahedra, edges with two equivalent Mn(2)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles are 52°. There are three inequivalent Cu sites. In the first Cu site, Cu(1) is bonded to one O(14), one O(2), one O(3), one O(4), one O(7), and one O(9) atom to form CuO6 octahedra that share corners with two equivalent Sn(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Sn(1)O6 octahedra, edges with two equivalent Mn(1)O6 octahedra, and edges with two equivalent Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles are 54°. In the second Cu site, Cu(2) is bonded to one O(16), one O(2), one O(3), one O(4), one O(8), and one O(9) atom to form CuO6 octahedra that share corners with two equivalent Sn(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Sn(1)O6 octahedra, edges with two equivalent Mn(1)O6 octahedra, and edges with two equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-55°. In the third Cu site, Cu(3) is bonded to one O(1), one O(11), one O(12), one O(13), one O(5), and one O(6) atom to form CuO6 octahedra that share corners with two equivalent Sn(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Sn(2)O6 octahedra, edges with two equivalent Mn(2)O6 octahedra, and edges with two equivalent Mn(3)O6 octahedra. The corner-sharing octahedral tilt angles are 55°. There are two inequivalent Sn sites. In the first Sn site, Sn(1) is bonded to one O(1), one O(10), one O(2), one O(6), one O(7), and one O(8) atom to form SnO6 octahedra that share corners with two equivalent Mn(2)O6 octahedra, corners with two equivalent Mn(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, corners with three equivalent Li(4)O4 tetrahedra,  an edgeedge with one Mn(1)O6 octahedra,  an edgeedge with one Cu(1)O6 octahedra, and  an edgeedge with one Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-55°. In the second Sn site, Sn(2) is bonded to one O(11), one O(12), one O(14), one O(15), one O(16), and one O(9) atom to form distorted SnO6 octahedra that share corners with two equivalent Mn(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra,  an edgeedge with one Mn(2)O6 octahedra,  an edgeedge with one Mn(3)O6 octahedra, and  an edgeedge with one Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 52-55°. There are sixteen inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one Mn(2), one Cu(3), and one Sn(1) atom. In the second O site, O(2) is bonded to one Li(4), one Cu(1), one Cu(2), and one Sn(1) atom to form distorted corner-sharing OLiCu2Sn tetrahedra. In the third O site, O(3) is bonded in a rectangular see-saw-like geometry to one Li(1), one Mn(1), one Cu(1), and one Cu(2) atom. In the fourth O site, O(4) is bonded to one Li(3), one Mn(1), one Cu(1), and one Cu(2) atom to form corner-sharing OLiMnCu2 tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), one Mn(2), one Mn(3), and one Cu(3) atom to form distorted OLiMn2Cu tetrahedra that share corners with two equivalent O(15)LiMn2Sn tetrahedra, corners with two equivalent O(11)LiMnCuSn tetrahedra, and corners with two equivalent O(12)LiMnCuSn tetrahedra. In the sixth O site, O(6) is bonded in a rectangular see-saw-like geometry to one Li(3), one Mn(3), one Cu(3), and one Sn(1) atom. In the seventh O site, O(7) is bonded in a distorted rectangular see-saw-like geometry to one Li(4), one Mn(1), one Cu(1), and one Sn(1) atom. In the eighth O site, O(8) is bonded in a distorted rectangular see-saw-like geometry to one Li(4), one Mn(1), one Cu(2), and one Sn(1) atom. In the ninth O site, O(9) is bonded in a rectangular see-saw-like geometry to one Li(2), one Cu(1), one Cu(2), and one Sn(2) atom. In the tenth O site, O(10) is bonded in a rectangular see-saw-like geometry to one Li(3), one Mn(2), one Mn(3), and one Sn(1) atom. In the eleventh O site, O(11) is bonded to one Li(1), one Mn(2), one Cu(3), and one Sn(2) atom to form distorted OLiMnCuSn tetrahedra that share  a cornercorner with one O(15)LiMn2Sn tetrahedra,  a cornercorner with one O(12)LiMnCuSn tetrahedra, corners with two equivalent O(5)LiMn2Cu tetrahedra,  an edgeedge with one O(15)LiMn2Sn tetrahedra, and  an edgeedge with one O(12)LiMnCuSn tetrahedra. In the twelfth O site, O(12) is bonded to one Li(1), one Mn(3), one Cu(3), and one Sn(2) atom to form distorted OLiMnCuSn tetrahedra that share  a cornercorner with one O(15)LiMn2Sn tetrahedra,  a cornercorner with one O(11)LiMnCuSn tetrahedra, corners with two equivalent O(5)LiMn2Cu tetrahedra,  an edgeedge with one O(15)LiMn2Sn tetrahedra, and  an edgeedge with one O(11)LiMnCuSn tetrahedra. In the thirteenth O site, O(13) is bonded in a distorted rectangular see-saw-like geometry to one Li(4), one Mn(2), one Mn(3), and one Cu(3) atom. In the fourteenth O site, O(14) is bonded in a rectangular see-saw-like geometry to one Li(2), one Mn(1), one Cu(1), and one Sn(2) atom. In the fifteenth O site, O(15) is bonded to one Li(1), one Mn(2), one Mn(3), and one Sn(2) atom to form distorted OLiMn2Sn tetrahedra that share  a cornercorner with one O(11)LiMnCuSn tetrahedra,  a cornercorner with one O(12)LiMnCuSn tetrahedra, corners with two equivalent O(5)LiMn2Cu tetrahedra,  an edgeedge with one O(11)LiMnCuSn tetrahedra, and  an edgeedge with one O(12)LiMnCuSn tetrahedra. In the sixteenth O site, O(16) is bonded in a rectangular see-saw-like geometry to one Li(2), one Mn(1), one Cu(2), and one Sn(2) atom. is represented by the CIF card [CIF]
data_Li4Mn3Cu3(SnO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.956
_cell_length_b   5.900
_cell_length_c   9.683
_cell_angle_alpha   89.976
_cell_angle_beta   89.097
_cell_angle_gamma   119.774
_symmetry_Int_Tables_number   1
_cell_volume   295.313
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.340  0.670  0.897  1.0
  Li  Li1  1  0.998  0.999  0.997  1.0
  Li  Li2  1  0.999  0.999  0.492  1.0
  Li  Li3  1  0.674  0.337  0.390  1.0
  Mn  Mn4  1  0.659  0.829  0.215  1.0
  Mn  Mn5  1  0.831  0.661  0.715  1.0
  Mn  Mn6  1  0.830  0.169  0.715  1.0
  Cu  Cu7  1  0.168  0.828  0.214  1.0
  Cu  Cu8  1  0.169  0.340  0.214  1.0
  Cu  Cu9  1  0.339  0.170  0.715  1.0
  Sn  Sn10  1  0.326  0.663  0.489  1.0
  Sn  Sn11  1  0.657  0.328  0.995  1.0
  O  O12  1  0.147  0.832  0.600  1.0
  O  O13  1  0.036  0.519  0.340  1.0
  O  O14  1  0.351  0.675  0.108  1.0
  O  O15  1  0.985  0.994  0.306  1.0
  O  O16  1  0.984  0.992  0.808  1.0
  O  O17  1  0.148  0.315  0.601  1.0
  O  O18  1  0.499  0.970  0.339  1.0
  O  O19  1  0.499  0.528  0.340  1.0
  O  O20  1  0.310  0.154  0.097  1.0
  O  O21  1  0.677  0.839  0.606  1.0
  O  O22  1  0.534  0.497  0.837  1.0
  O  O23  1  0.533  0.036  0.837  1.0
  O  O24  1  0.685  0.342  0.610  1.0
  O  O25  1  0.827  0.677  0.100  1.0
  O  O26  1  0.969  0.484  0.831  1.0
  O  O27  1  0.827  0.150  0.100  1.0
[/CIF]
.
The crystal structure described by Li4Mn3Cu3(SnO8)2 is Spinel-derived structured and crystallizes in the triclinic P1 space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(11), one O(12), one O(15), and one O(3) atom to form LiO4 tetrahedra that share  a cornercorner with one Mn(1)O6 octahedra,  a cornercorner with one Cu(1)O6 octahedra,  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Mn(2)O6 octahedra, corners with two equivalent Mn(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, and corners with three equivalent Sn(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 55-63°. In the second Li site, Li(2) is bonded in a rectangular see-saw-like geometry to one O(14), one O(16), one O(5), and one O(9) atom. In the third Li site, Li(3) is bonded in a rectangular see-saw-like geometry to one O(1), one O(10), one O(4), and one O(6) atom. In the fourth Li site, Li(4) is bonded to one O(13), one O(2), one O(7), and one O(8) atom to form LiO4 tetrahedra that share  a cornercorner with one Mn(2)O6 octahedra,  a cornercorner with one Mn(3)O6 octahedra,  a cornercorner with one Cu(3)O6 octahedra, corners with two equivalent Mn(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, and corners with three equivalent Sn(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 57-63°. There are three inequivalent Mn sites. In the first Mn site, Mn(1) is bonded to one O(14), one O(16), one O(3), one O(4), one O(7), and one O(8) atom to form MnO6 octahedra that share corners with two equivalent Sn(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Sn(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, and edges with two equivalent Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles are 52°. In the second Mn site, Mn(2) is bonded to one O(1), one O(10), one O(11), one O(13), one O(15), and one O(5) atom to form MnO6 octahedra that share corners with two equivalent Sn(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Sn(2)O6 octahedra, edges with two equivalent Mn(3)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-52°. In the third Mn site, Mn(3) is bonded to one O(10), one O(12), one O(13), one O(15), one O(5), and one O(6) atom to form MnO6 octahedra that share corners with two equivalent Sn(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Sn(2)O6 octahedra, edges with two equivalent Mn(2)O6 octahedra, and edges with two equivalent Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles are 52°. There are three inequivalent Cu sites. In the first Cu site, Cu(1) is bonded to one O(14), one O(2), one O(3), one O(4), one O(7), and one O(9) atom to form CuO6 octahedra that share corners with two equivalent Sn(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Sn(1)O6 octahedra, edges with two equivalent Mn(1)O6 octahedra, and edges with two equivalent Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles are 54°. In the second Cu site, Cu(2) is bonded to one O(16), one O(2), one O(3), one O(4), one O(8), and one O(9) atom to form CuO6 octahedra that share corners with two equivalent Sn(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one Sn(1)O6 octahedra, edges with two equivalent Mn(1)O6 octahedra, and edges with two equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-55°. In the third Cu site, Cu(3) is bonded to one O(1), one O(11), one O(12), one O(13), one O(5), and one O(6) atom to form CuO6 octahedra that share corners with two equivalent Sn(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one Sn(2)O6 octahedra, edges with two equivalent Mn(2)O6 octahedra, and edges with two equivalent Mn(3)O6 octahedra. The corner-sharing octahedral tilt angles are 55°. There are two inequivalent Sn sites. In the first Sn site, Sn(1) is bonded to one O(1), one O(10), one O(2), one O(6), one O(7), and one O(8) atom to form SnO6 octahedra that share corners with two equivalent Mn(2)O6 octahedra, corners with two equivalent Mn(3)O6 octahedra, corners with two equivalent Cu(3)O6 octahedra, corners with three equivalent Li(4)O4 tetrahedra,  an edgeedge with one Mn(1)O6 octahedra,  an edgeedge with one Cu(1)O6 octahedra, and  an edgeedge with one Cu(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-55°. In the second Sn site, Sn(2) is bonded to one O(11), one O(12), one O(14), one O(15), one O(16), and one O(9) atom to form distorted SnO6 octahedra that share corners with two equivalent Mn(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra,  an edgeedge with one Mn(2)O6 octahedra,  an edgeedge with one Mn(3)O6 octahedra, and  an edgeedge with one Cu(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 52-55°. There are sixteen inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one Mn(2), one Cu(3), and one Sn(1) atom. In the second O site, O(2) is bonded to one Li(4), one Cu(1), one Cu(2), and one Sn(1) atom to form distorted corner-sharing OLiCu2Sn tetrahedra. In the third O site, O(3) is bonded in a rectangular see-saw-like geometry to one Li(1), one Mn(1), one Cu(1), and one Cu(2) atom. In the fourth O site, O(4) is bonded to one Li(3), one Mn(1), one Cu(1), and one Cu(2) atom to form corner-sharing OLiMnCu2 tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), one Mn(2), one Mn(3), and one Cu(3) atom to form distorted OLiMn2Cu tetrahedra that share corners with two equivalent O(15)LiMn2Sn tetrahedra, corners with two equivalent O(11)LiMnCuSn tetrahedra, and corners with two equivalent O(12)LiMnCuSn tetrahedra. In the sixth O site, O(6) is bonded in a rectangular see-saw-like geometry to one Li(3), one Mn(3), one Cu(3), and one Sn(1) atom. In the seventh O site, O(7) is bonded in a distorted rectangular see-saw-like geometry to one Li(4), one Mn(1), one Cu(1), and one Sn(1) atom. In the eighth O site, O(8) is bonded in a distorted rectangular see-saw-like geometry to one Li(4), one Mn(1), one Cu(2), and one Sn(1) atom. In the ninth O site, O(9) is bonded in a rectangular see-saw-like geometry to one Li(2), one Cu(1), one Cu(2), and one Sn(2) atom. In the tenth O site, O(10) is bonded in a rectangular see-saw-like geometry to one Li(3), one Mn(2), one Mn(3), and one Sn(1) atom. In the eleventh O site, O(11) is bonded to one Li(1), one Mn(2), one Cu(3), and one Sn(2) atom to form distorted OLiMnCuSn tetrahedra that share  a cornercorner with one O(15)LiMn2Sn tetrahedra,  a cornercorner with one O(12)LiMnCuSn tetrahedra, corners with two equivalent O(5)LiMn2Cu tetrahedra,  an edgeedge with one O(15)LiMn2Sn tetrahedra, and  an edgeedge with one O(12)LiMnCuSn tetrahedra. In the twelfth O site, O(12) is bonded to one Li(1), one Mn(3), one Cu(3), and one Sn(2) atom to form distorted OLiMnCuSn tetrahedra that share  a cornercorner with one O(15)LiMn2Sn tetrahedra,  a cornercorner with one O(11)LiMnCuSn tetrahedra, corners with two equivalent O(5)LiMn2Cu tetrahedra,  an edgeedge with one O(15)LiMn2Sn tetrahedra, and  an edgeedge with one O(11)LiMnCuSn tetrahedra. In the thirteenth O site, O(13) is bonded in a distorted rectangular see-saw-like geometry to one Li(4), one Mn(2), one Mn(3), and one Cu(3) atom. In the fourteenth O site, O(14) is bonded in a rectangular see-saw-like geometry to one Li(2), one Mn(1), one Cu(1), and one Sn(2) atom. In the fifteenth O site, O(15) is bonded to one Li(1), one Mn(2), one Mn(3), and one Sn(2) atom to form distorted OLiMn2Sn tetrahedra that share  a cornercorner with one O(11)LiMnCuSn tetrahedra,  a cornercorner with one O(12)LiMnCuSn tetrahedra, corners with two equivalent O(5)LiMn2Cu tetrahedra,  an edgeedge with one O(11)LiMnCuSn tetrahedra, and  an edgeedge with one O(12)LiMnCuSn tetrahedra. In the sixteenth O site, O(16) is bonded in a rectangular see-saw-like geometry to one Li(2), one Mn(1), one Cu(2), and one Sn(2) atom. is represented by the CIF card [CIF]
data_Li4Mn3Cu3(SnO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.956
_cell_length_b   5.900
_cell_length_c   9.683
_cell_angle_alpha   89.976
_cell_angle_beta   89.097
_cell_angle_gamma   119.774
_symmetry_Int_Tables_number   1
_cell_volume   295.313
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.340  0.670  0.897  1.0
  Li  Li1  1  0.998  0.999  0.997  1.0
  Li  Li2  1  0.999  0.999  0.492  1.0
  Li  Li3  1  0.674  0.337  0.390  1.0
  Mn  Mn4  1  0.659  0.829  0.215  1.0
  Mn  Mn5  1  0.831  0.661  0.715  1.0
  Mn  Mn6  1  0.830  0.169  0.715  1.0
  Cu  Cu7  1  0.168  0.828  0.214  1.0
  Cu  Cu8  1  0.169  0.340  0.214  1.0
  Cu  Cu9  1  0.339  0.170  0.715  1.0
  Sn  Sn10  1  0.326  0.663  0.489  1.0
  Sn  Sn11  1  0.657  0.328  0.995  1.0
  O  O12  1  0.147  0.832  0.600  1.0
  O  O13  1  0.036  0.519  0.340  1.0
  O  O14  1  0.351  0.675  0.108  1.0
  O  O15  1  0.985  0.994  0.306  1.0
  O  O16  1  0.984  0.992  0.808  1.0
  O  O17  1  0.148  0.315  0.601  1.0
  O  O18  1  0.499  0.970  0.339  1.0
  O  O19  1  0.499  0.528  0.340  1.0
  O  O20  1  0.310  0.154  0.097  1.0
  O  O21  1  0.677  0.839  0.606  1.0
  O  O22  1  0.534  0.497  0.837  1.0
  O  O23  1  0.533  0.036  0.837  1.0
  O  O24  1  0.685  0.342  0.610  1.0
  O  O25  1  0.827  0.677  0.100  1.0
  O  O26  1  0.969  0.484  0.831  1.0
  O  O27  1  0.827  0.150  0.100  1.0
[/CIF]
.